#------------------------------------------------------------------------------
#$Date: 2023-12-06 15:08:03 +0200 (Wed, 06 Dec 2023) $
#$Revision: 288072 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/54/73/1547373.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1547373
loop_
_publ_author_name
'Nobuo Ishizawa'
'Hayato Setoguchi'
'Kazumichi Yanagisawa'
_publ_section_title
;
 Structural evolution of calcite at high temperatures: Phase V unveiled
;
_journal_name_full               'Scientific Reports'
_journal_page_first              2832
_journal_paper_doi               10.1038/srep02832
_journal_volume                  3
_journal_year                    2013
_chemical_absolute_configuration .
_chemical_formula_sum            'C Ca O3'
_chemical_formula_weight         100.1
_space_group_IT_number           167
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.9745
_cell_length_b                   4.9745
_cell_length_c                   17.4912(3)
_cell_measurement_temperature    1037
_cell_volume                     374.843(6)
_diffrn_ambient_temperature      1037
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0272
_diffrn_reflns_av_sigmaI/netI    0.0136
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            1333
_diffrn_reflns_theta_full        35
_diffrn_reflns_theta_max         35
_diffrn_reflns_theta_min         5.28
_exptl_absorpt_coefficient_mu    2.239
_exptl_crystal_density_diffrn    2.6595
_exptl_crystal_F_000             300
_refine_diff_density_max         0.14
_refine_diff_density_min         -0.20
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    1.72
_refine_ls_goodness_of_fit_ref   1.63
_refine_ls_number_constraints    9
_refine_ls_number_parameters     15
_refine_ls_number_reflns         188
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0243
_refine_ls_R_factor_gt           0.0217
_refine_ls_shift/su_max          0.0022
_refine_ls_shift/su_mean         0.0007
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0250
_refine_ls_wR_factor_ref         0.0256
_reflns_number_gt                163
_reflns_number_total             188
_reflns_threshold_expression     I>3σ(I)
_cod_data_source_file            srep02832-s3-Copie2.cif
_cod_data_source_block           1037K_hs30_h740_IV_anharm
_cod_depositor_comments
;
The following automatic conversions were performed:

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to the built-in table from CIF Core dictionary named 'cif_core.dic'
version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 5376 2017-05-30 11:51:03Z andrius 

The following automatic conversions were performed:

data name '_atom_site_site_symmetry_mutiplicity' was replaced with
'_atom_site_site_symmetry_multiplicity' as specified in the
replacement file 'data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 9268 2022-04-12 08:56:07Z antanas 
;
_cod_original_sg_symbol_Hall     '-R 3;-2"c'
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        'C1 Ca1 O3'
_cod_database_code               1547373
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 -y,x-y,z
3 -x+y,-x,z
4 y,x,-z+1/2
5 x-y,-y,-z+1/2
6 -x,-x+y,-z+1/2
7 -x,-y,-z
8 y,-x+y,-z
9 x-y,x,-z
10 -y,-x,z+1/2
11 -x+y,y,z+1/2
12 x,x-y,z+1/2
13 x+2/3,y+1/3,z+1/3
14 -y+2/3,x-y+1/3,z+1/3
15 -x+y+2/3,-x+1/3,z+1/3
16 y+2/3,x+1/3,-z+5/6
17 x-y+2/3,-y+1/3,-z+5/6
18 -x+2/3,-x+y+1/3,-z+5/6
19 -x+2/3,-y+1/3,-z+1/3
20 y+2/3,-x+y+1/3,-z+1/3
21 x-y+2/3,x+1/3,-z+1/3
22 -y+2/3,-x+1/3,z+5/6
23 -x+y+2/3,y+1/3,z+5/6
24 x+2/3,x-y+1/3,z+5/6
25 x+1/3,y+2/3,z+2/3
26 -y+1/3,x-y+2/3,z+2/3
27 -x+y+1/3,-x+2/3,z+2/3
28 y+1/3,x+2/3,-z+1/6
29 x-y+1/3,-y+2/3,-z+1/6
30 -x+1/3,-x+y+2/3,-z+1/6
31 -x+1/3,-y+2/3,-z+2/3
32 y+1/3,-x+y+2/3,-z+2/3
33 x-y+1/3,x+2/3,-z+2/3
34 -y+1/3,-x+2/3,z+1/6
35 -x+y+1/3,y+2/3,z+1/6
36 x+1/3,x-y+2/3,z+1/6
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ca1 Ca 0 0 0 Uani 0.04567(16) 6 1 d . . .
C1 C 0 0 0.25 Uani 0.0384(4) 6 1 d . . .
O1 O 0.2482(4) 0 0.25 Uani 0.0822(7) 18 0.989(4) d . . .
O2 O -0.2482(4) 0 0.25 Uani 0.0822(7) 18 0.011(4) d . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C 0.0033 0.0016 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ca 0.2262 0.3064 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
O 0.0106 0.0060 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
Ca1 Ca1 . 16_444 4.09230(7)
Ca1 Ca1 . 16_454 4.09230(7)
Ca1 Ca1 . 16_554 4.09230(7)
Ca1 Ca1 . 28_445 4.09230(7)
Ca1 Ca1 . 28_545 4.09230(7)
Ca1 Ca1 . 28_555 4.09230(7)
Ca1 C1 . 25_444 3.22074(2)
Ca1 C1 . 25_544 3.22074(2)
Ca1 C1 . 25_554 3.22074(2)
Ca1 C1 . 19_445 3.22074(2)
Ca1 C1 . 19_455 3.22074(2)
Ca1 C1 . 19_555 3.22074(2)
Ca1 O1 . 25_444 2.3991(11)
Ca1 O1 . 26_544 2.3991(11)
Ca1 O1 . 27_554 2.3991(18)
Ca1 O1 . 19_555 2.3991(11)
Ca1 O1 . 20_455 2.3991(11)
Ca1 O1 . 21_445 2.3991(18)
Ca1 O2 . 25_544 2.3991(11)
Ca1 O2 . 26_554 2.3991(11)
Ca1 O2 . 27_444 2.3991(18)
Ca1 O2 . 19_455 2.3991(11)
Ca1 O2 . 20_445 2.3991(11)
Ca1 O2 . 21_555 2.3991(18)
C1 O1 . . 1.235(2)
C1 O1 . 2_555 1.235(2)
C1 O1 . 3_555 1.2346(15)
C1 O2 . . 1.235(2)
C1 O2 . 2_555 1.235(2)
C1 O2 . 3_555 1.2346(15)
O1 O2 . 2_555 1.2346(15)
O1 O2 . 3_555 1.235(3)
loop_
_jana_atom_site_adp_c_label
_jana_atom_site_adp_c_type_symbol
_jana_atom_site_adp_c_111
_jana_atom_site_adp_c_112
_jana_atom_site_adp_c_113
_jana_atom_site_adp_c_122
_jana_atom_site_adp_c_123
_jana_atom_site_adp_c_133
_jana_atom_site_adp_c_222
_jana_atom_site_adp_c_223
_jana_atom_site_adp_c_233
_jana_atom_site_adp_c_333
O1 O -0.058(5) -0.058(5) 0.0064(8) -0.058(5) 0.0064(8) -0.0018(2) 0 0 0 0
O2 O -0.058(5) -0.058(5) 0.0064(8) -0.058(5) 0.0064(8) -0.0018(2) 0 0 0 0
